#------------------------------------------------------------------------------
#$Date: 2016-03-24 14:36:54 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179669 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/22/4512294.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4512294
loop_
_publ_author_name
'Zhao, Jun-Wei'
'Cao, Jing'
'Li, Yan-Zhou'
'Zhang, Jing'
'Chen, Li-Juan'
_publ_section_title
;
 First Tungstoantimonate-Based Transition-Metal--Lanthanide Heterometallic
 Hybrids Functionalized by Amino Acid Ligands
;
_journal_issue                   12
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              6217
_journal_paper_doi               10.1021/cg5007988
_journal_volume                  14
_journal_year                    2014
_chemical_formula_sum            'C8 H110 Fe4 N2 O118 Sb2 Sm2 W18'
_chemical_formula_weight         6199.88
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                106.9910(10)
_cell_angle_beta                 99.9670(10)
_cell_angle_gamma                96.7560(10)
_cell_formula_units_Z            1
_cell_length_a                   12.6058(5)
_cell_length_b                   13.5742(5)
_cell_length_c                   16.2643(7)
_cell_measurement_reflns_used    8995
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.72
_cell_volume                     2579.25(18)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0395
_diffrn_reflns_av_sigmaI/netI    0.0791
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            13321
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.72
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    22.287
_exptl_absorpt_correction_T_max  0.3482
_exptl_absorpt_correction_T_min  0.0475
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'green yellow'
_exptl_crystal_density_diffrn    3.992
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'cubic block'
_exptl_crystal_F_000             2778
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.06
_refine_diff_density_max         4.494
_refine_diff_density_min         -3.384
_refine_diff_density_rms         0.496
_refine_ls_extinction_coef       0.00015(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     629
_refine_ls_number_reflns         8995
_refine_ls_number_restraints     25
_refine_ls_restrained_S_all      1.025
_refine_ls_R_factor_all          0.0633
_refine_ls_R_factor_gt           0.0539
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0738P)²+55.0026P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1388
_refine_ls_wR_factor_ref         0.1448
_reflns_number_gt                7690
_reflns_number_total             8995
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg5007988_si_002.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4512292--4512298.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4512294
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sb1 Sb 0.35723(8) 0.36011(8) 0.34606(7) 0.0095(2) Uani 1 1 d .
W1 W 0.35667(5) 0.61553(5) 0.47127(5) 0.01275(17) Uani 1 1 d .
W2 W 0.09793(5) 0.48691(5) 0.37938(5) 0.01518(18) Uani 1 1 d .
W3 W 0.24850(5) 0.57419(5) 0.25615(5) 0.01575(18) Uani 1 1 d .
W4 W 0.46862(5) 0.43876(5) 0.17985(5) 0.01446(18) Uani 1 1 d .
W5 W 0.21485(5) 0.31108(5) 0.09634(5) 0.01492(18) Uani 1 1 d .
W6 W 0.04562(5) 0.21523(5) 0.23233(5) 0.01390(18) Uani 1 1 d .
W7 W 0.15213(5) 0.25524(5) 0.44330(5) 0.01554(18) Uani 1 1 d .
W8 W 0.24661(5) 0.09005(5) 0.29009(5) 0.01587(18) Uani 1 1 d .
W9 W 0.41467(5) 0.18402(5) 0.15353(5) 0.01692(18) Uani 1 1 d .
Fe1 Fe 0.38008(18) 0.43062(18) 0.60037(16) 0.0136(5) Uani 1 1 d .
O1W O 0.2402(9) 0.4517(9) 0.6511(9) 0.024(3) Uani 1 1 d .
O2W O 0.4090(11) 0.3194(10) 0.6631(9) 0.030(3) Uani 1 1 d .
O5W O 0.043(2) 0.3991(19) -0.1197(17) 0.092 Uiso 1 1 d .
O6W O 0.2761(15) 0.3783(15) -0.0946(13) 0.066(6) Uani 1 1 d .
O7W O 0.077(2) 0.343(2) -0.265(2) 0.115(9) Uiso 1 1 d .
O8W O -0.0561(19) 0.1844(18) -0.2775(16) 0.084 Uiso 1 1 d .
O9W O 0.2402(18) 0.2249(19) -0.2730(15) 0.081(7) Uani 1 1 d .
O10W O 0.073(3) 0.058(3) -0.283(2) 0.136(11) Uiso 1 1 d .
O11W O 0.017(2) 0.105(2) -0.1233(19) 0.108(8) Uani 1 1 d U
O12W O 0.2566(17) 0.1446(15) -0.1186(14) 0.074(6) Uani 1 1 d .
O13W O 0.205(5) 0.018(4) 0.577(4) 0.11(2) Uani 0.50 1 d P
O14W O 0.351(3) 0.8812(17) 0.4005(17) 0.119(11) Uani 1 1 d .
O15W O -0.082(4) 0.471(3) -0.002(3) 0.095(17) Uani 0.50 1 d P
O16W O -0.1320(19) 0.1988(19) -0.0112(14) 0.082(7) Uani 1 1 d .
O17W O 0.1181(17) 0.0037(16) 0.0058(14) 0.075(6) Uani 1 1 d .
O18W O -0.0926(18) 0.3943(17) 0.1303(16) 0.082(7) Uani 1 1 d .
O19W O 0.2569(16) 0.6448(16) 0.7716(15) 0.076(6) Uani 1 1 d .
O20W O -0.120(2) 0.199(2) 0.554(2) 0.119(10) Uani 1 1 d .
O21W O 0.1647(12) 0.7133(12) 0.6307(11) 0.046(4) Uani 1 1 d .
O23W O 0.300(3) 0.944(3) 0.857(3) 0.159(13) Uiso 1 1 d .
O22W O 0.680(5) 0.123(5) 0.086(5) 0.13(2) Uiso 0.50 1 d P
O24W O 0.388(3) 1.048(3) 0.824(3) 0.063(10) Uani 0.50 1 d PU
O25W O 0.3774(19) 0.1328(15) 0.5425(14) 0.079(7) Uani 1 1 d .
O1 O 0.4834(9) 0.5920(9) 0.4379(9) 0.022(3) Uani 1 1 d .
O2 O 0.2739(9) 0.4789(8) 0.3531(8) 0.014(2) Uani 1 1 d .
O3 O 0.3560(9) 0.5309(9) 0.5371(8) 0.018(3) Uani 1 1 d .
O4 O 0.3947(10) 0.7415(9) 0.5513(9) 0.025(3) Uani 1 1 d .
O5 O 0.3165(11) 0.6690(10) 0.3682(9) 0.009(3) Uiso 0.80 1 d P
O5' O 0.355(4) 0.634(4) 0.340(4) 0.010 Uiso 0.20 1 d P
O6 O 0.1924(11) 0.6010(11) 0.4647(9) 0.011 Uiso 0.80 1 d P
O6' O 0.210(4) 0.553(4) 0.472(4) 0.010 Uiso 0.20 1 d P
O7 O -0.0262(10) 0.5185(9) 0.3982(9) 0.025(3) Uani 1 1 d .
O8 O 0.1235(9) 0.3961(8) 0.4448(8) 0.016(3) Uani 1 1 d .
O9 O 0.0512(8) 0.3626(8) 0.2748(8) 0.013(2) Uani 1 1 d .
O10 O 0.1132(10) 0.5606(11) 0.2937(9) 0.010 Uiso 0.80 1 d P
O10' O 0.101(4) 0.498(4) 0.257(4) 0.010 Uiso 0.20 1 d P
O11 O 0.2220(9) 0.6591(10) 0.1978(9) 0.026(3) Uani 1 1 d .
O12 O 0.1855(9) 0.4382(9) 0.1668(8) 0.020(3) Uani 1 1 d .
O13 O 0.3857(9) 0.5454(9) 0.2290(8) 0.018(3) Uiso 1 1 d .
O14 O 0.3454(8) 0.3297(8) 0.2169(7) 0.010(2) Uiso 1 1 d .
O15 O 0.5564(10) 0.5085(10) 0.1383(10) 0.030(3) Uani 1 1 d .
O16 O 0.5004(9) 0.2997(9) 0.1354(8) 0.021(3) Uani 1 1 d .
O17 O 0.5437(10) 0.4600(9) 0.2921(8) 0.019(3) Uani 1 1 d .
O18 O 0.3417(9) 0.3948(9) 0.0839(8) 0.020(3) Uani 1 1 d .
O19 O 0.1366(10) 0.2913(10) -0.0079(9) 0.026(3) Uani 1 1 d .
O20 O 0.2901(9) 0.1955(9) 0.0671(9) 0.021(3) Uani 1 1 d .
O21 O 0.1188(9) 0.2361(8) 0.1436(7) 0.014(2) Uani 1 1 d .
O22 O -0.0860(9) 0.1701(9) 0.1716(8) 0.020(3) Uani 1 1 d U
O23 O 0.2202(9) 0.2565(9) 0.3217(8) 0.017(3) Uani 1 1 d .
O24 O 0.0981(9) 0.0860(9) 0.2223(9) 0.021(3) Uani 1 1 d .
O25 O 0.0233(9) 0.2128(8) 0.3443(8) 0.018(3) Uani 1 1 d .
O26 O 0.0893(9) 0.2395(9) 0.5236(8) 0.020(3) Uiso 1 1 d .
O27 O 0.1820(9) 0.1179(9) 0.3950(8) 0.017(3) Uani 1 1 d .
O28 O 0.2915(9) 0.3159(8) 0.5036(8) 0.016(2) Uani 1 1 d .
O29 O 0.2352(10) -0.0450(9) 0.2683(9) 0.024(3) Uani 1 1 d .
O30 O 0.3017(10) 0.1077(9) 0.1935(8) 0.020(3) Uani 1 1 d .
O31 O 0.3811(9) 0.1410(9) 0.3621(8) 0.022(3) Uani 1 1 d .
O32 O 0.4576(11) 0.0802(10) 0.0841(9) 0.028(3) Uani 1 1 d .
O33 O 0.5052(9) 0.2070(9) 0.2618(8) 0.019(3) Uani 1 1 d .
Sm1 Sm 0.11640(8) 0.23653(8) -0.17046(7) 0.0299(3) Uani 1 1 d .
Fe2 Fe 0.5330(2) 0.13424(19) 0.34602(18) 0.0192(6) Uani 1 1 d .
O3W O 0.6871(10) 0.1192(11) 0.3230(10) 0.034(3) Uani 1 1 d .
O4W O 0.5493(13) 0.0445(10) 0.4298(10) 0.041(4) Uani 1 1 d .
O34 O 0.4800(11) -0.0070(9) 0.2484(9) 0.028(3) Uani 1 1 d .
O35 O 0.5655(19) -0.1283(18) 0.2669(17) 0.088 Uiso 1 1 d .
H35A H 0.5857 -0.0978 0.3200 0.131 Uiso 1 1 calc R
O36 O 0.5192(19) -0.2102(18) 0.0526(16) 0.083 Uiso 1 1 d .
H36A H 0.5569 -0.1532 0.0821 0.125 Uiso 1 1 calc R
N1 N 0.341(3) -0.115(3) 0.110(3) 0.120(12) Uiso 1 1 d D
H1A H 0.3345 -0.1250 0.0543 0.144 Uiso 1 1 calc R
H1B H 0.3095 -0.0690 0.1403 0.144 Uiso 1 1 calc R
C1 C 0.491(3) -0.084(3) 0.233(3) 0.081 Uiso 1 1 d .
C2 C 0.406(3) -0.177(3) 0.153(2) 0.082 Uiso 1 1 d D
H2A H 0.3567 -0.2105 0.1808 0.098 Uiso 1 1 calc R
C3 C 0.464(3) -0.257(2) 0.111(3) 0.098(14) Uani 1 1 d .
H3A H 0.5121 -0.2817 0.1516 0.118 Uiso 1 1 calc R
C4 C 0.365(4) -0.351(4) 0.034(3) 0.131(17) Uani 1 1 d U
H4A H 0.3989 -0.4040 0.0009 0.197 Uiso 1 1 calc R
H4D H 0.3250 -0.3199 -0.0043 0.197 Uiso 1 1 calc R
H4B H 0.3166 -0.3810 0.0633 0.197 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O14 Sb1 O23 89.9(5) . .
O14 Sb1 O2 92.1(4) . .
O23 Sb1 O2 92.1(5) . .
O4 W1 O3 102.7(6) . .
O4 W1 O1 102.8(6) . .
O3 W1 O1 97.0(5) . .
O4 W1 O6' 109.8(17) . .
O3 W1 O6' 67.0(17) . .
O1 W1 O6' 146.0(17) . .
O4 W1 O5 94.9(6) . .
O3 W1 O5 159.8(5) . .
O1 W1 O5 88.6(6) . .
O6' W1 O5 97.8(17) . .
O4 W1 O6 97.0(6) . .
O3 W1 O6 85.9(5) . .
O1 W1 O6 158.8(6) . .
O6' W1 O6 21.2(15) . .
O5 W1 O6 82.1(6) . .
O4 W1 O5' 108.0(15) . .
O3 W1 O5' 148.4(15) . .
O1 W1 O5' 69.1(15) . .
O6' W1 O5' 108(2) . .
O5 W1 O5' 21.8(13) . .
O6 W1 O5' 97.7(14) . .
O4 W1 O2 163.7(5) . .
O3 W1 O2 89.1(5) . .
O1 W1 O2 86.6(5) . .
O6' W1 O2 64.3(17) . .
O5 W1 O2 71.8(5) . .
O6 W1 O2 72.4(5) . .
O5' W1 O2 62.7(14) . .
O7 W2 O6' 112.8(18) . .
O7 W2 O6 99.9(6) . .
O6' W2 O6 23.2(17) . .
O7 W2 O8 102.6(6) . .
O6' W2 O8 72.2(18) . .
O6 W2 O8 93.5(6) . .
O7 W2 O9 101.4(5) . .
O6' W2 O9 143.0(18) . .
O6 W2 O9 158.0(5) . .
O8 W2 O9 87.3(5) . .
O7 W2 O10 97.2(6) . .
O6' W2 O10 104.6(18) . .
O6 W2 O10 87.9(6) . .
O8 W2 O10 159.6(5) . .
O9 W2 O10 84.0(5) . .
O7 W2 O10' 104.5(15) . .
O6' W2 O10' 121(2) . .
O6 W2 O10' 109.3(16) . .
O8 W2 O10' 140.6(16) . .
O9 W2 O10' 59.7(16) . .
O10 W2 O10' 24.6(14) . .
O7 W2 O2 168.3(5) . .
O6' W2 O2 63.8(18) . .
O6 W2 O2 72.9(5) . .
O8 W2 O2 87.2(4) . .
O9 W2 O2 85.2(4) . .
O10 W2 O2 73.7(5) . .
O10' W2 O2 70.4(14) . .
O5' W3 O11 108.0(18) . .
O5' W3 O5 26.0(19) . .
O11 W3 O5 100.8(6) . .
O5' W3 O13 67(2) . .
O11 W3 O13 99.8(5) . .
O5 W3 O13 92.4(6) . .
O5' W3 O10 113(2) . .
O11 W3 O10 98.7(6) . .
O5 W3 O10 89.9(6) . .
O13 W3 O10 160.5(5) . .
O5' W3 O12 141.9(19) . .
O11 W3 O12 101.7(6) . .
O5 W3 O12 157.4(5) . .
O13 W3 O12 85.4(5) . .
O10 W3 O12 85.0(6) . .
O5' W3 O10' 129(3) . .
O11 W3 O10' 106.1(15) . .
O5 W3 O10' 111.3(17) . .
O13 W3 O10' 140.2(16) . .
O10 W3 O10' 25.0(15) . .
O12 W3 O10' 60.3(17) . .
O5' W3 O2 68.9(18) . .
O11 W3 O2 170.5(5) . .
O5 W3 O2 72.3(5) . .
O13 W3 O2 87.3(4) . .
O10 W3 O2 75.0(5) . .
O12 W3 O2 85.1(4) . .
O10' W3 O2 71.2(15) . .
O15 W4 O17 103.7(6) . .
O15 W4 O18 100.4(6) . .
O17 W4 O18 155.3(5) . .
O15 W4 O16 101.1(6) . .
O17 W4 O16 93.7(5) . .
O18 W4 O16 86.8(5) . .
O15 W4 O13 100.5(6) . .
O17 W4 O13 88.0(5) . .
O18 W4 O13 82.4(5) . .
O16 W4 O13 157.3(5) . .
O15 W4 O14 172.4(6) . .
O17 W4 O14 82.4(4) . .
O18 W4 O14 74.0(4) . .
O16 W4 O14 73.7(4) . .
O13 W4 O14 84.1(4) . .
O19 W5 O12 104.5(5) . .
O19 W5 O21 101.6(5) . .
O12 W5 O21 89.7(5) . .
O19 W5 O20 98.3(6) . .
O12 W5 O20 156.7(5) . .
O21 W5 O20 90.7(5) . .
O19 W5 O18 96.4(6) . .
O12 W5 O18 86.0(5) . .
O21 W5 O18 162.0(5) . .
O20 W5 O18 86.4(5) . .
O19 W5 O14 167.9(5) . .
O12 W5 O14 83.6(4) . .
O21 W5 O14 87.2(4) . .
O20 W5 O14 73.1(5) . .
O18 W5 O14 74.9(4) . .
O22 W6 O25 99.7(5) . .
O22 W6 O9 102.7(5) . .
O25 W6 O9 87.0(5) . .
O22 W6 O21 100.4(5) . .
O25 W6 O21 160.0(5) . .
O9 W6 O21 88.3(5) . .
O22 W6 O24 100.9(5) . .
O25 W6 O24 86.3(5) . .
O9 W6 O24 156.2(5) . .
O21 W6 O24 90.3(5) . .
O22 W6 O23 172.0(5) . .
O25 W6 O23 75.1(4) . .
O9 W6 O23 83.3(4) . .
O21 W6 O23 85.0(4) . .
O24 W6 O23 72.9(4) . .
O26 W7 O28 102.8(5) . .
O26 W7 O27 101.0(5) . .
O28 W7 O27 96.6(5) . .
O26 W7 O25 99.0(5) . .
O28 W7 O25 157.1(5) . .
O27 W7 O25 85.9(5) . .
O26 W7 O8 99.7(5) . .
O28 W7 O8 88.3(5) . .
O27 W7 O8 157.0(5) . .
O25 W7 O8 81.2(5) . .
O26 W7 O23 172.0(5) . .
O28 W7 O23 84.2(5) . .
O27 W7 O23 74.0(4) . .
O25 W7 O23 74.6(4) . .
O8 W7 O23 84.2(5) . .
O29 W8 O31 103.1(6) . .
O29 W8 O30 101.2(6) . .
O31 W8 O30 90.8(5) . .
O29 W8 O27 96.7(5) . .
O31 W8 O27 89.0(5) . .
O30 W8 O27 161.6(5) . .
O29 W8 O24 96.3(5) . .
O31 W8 O24 160.4(5) . .
O30 W8 O24 87.7(5) . .
O27 W8 O24 86.4(5) . .
O29 W8 O23 166.4(5) . .
O31 W8 O23 86.9(5) . .
O30 W8 O23 87.6(5) . .
O27 W8 O23 74.0(4) . .
O24 W8 O23 73.5(4) . .
O32 W9 O33 103.6(6) . .
O32 W9 O16 100.0(6) . .
O33 W9 O16 91.6(5) . .
O32 W9 O20 97.6(6) . .
O33 W9 O20 158.3(5) . .
O16 W9 O20 88.9(5) . .
O32 W9 O30 100.5(5) . .
O33 W9 O30 87.4(5) . .
O16 W9 O30 159.1(5) . .
O20 W9 O30 84.6(5) . .
O32 W9 O14 167.2(5) . .
O33 W9 O14 87.9(5) . .
O16 W9 O14 73.9(4) . .
O20 W9 O14 71.4(4) . .
O30 W9 O14 85.2(4) . .
O28 Fe1 O17 171.9(5) . 2_666
O28 Fe1 O3 92.4(5) . .
O17 Fe1 O3 92.4(5) 2_666 .
O28 Fe1 O1 94.0(5) . 2_666
O17 Fe1 O1 92.2(5) 2_666 2_666
O3 Fe1 O1 92.3(5) . 2_666
O28 Fe1 O2W 86.1(5) . .
O17 Fe1 O2W 89.3(5) 2_666 .
O3 Fe1 O2W 177.3(6) . .
O1 Fe1 O2W 85.4(5) 2_666 .
O28 Fe1 O1W 88.2(5) . .
O17 Fe1 O1W 85.2(5) 2_666 .
O3 Fe1 O1W 92.0(5) . .
O1 Fe1 O1W 175.0(5) 2_666 .
O2W Fe1 O1W 90.3(6) . .
W1 O1 Fe1 178.2(7) . 2_666
Sb1 O2 W1 109.6(5) . .
Sb1 O2 W3 128.1(6) . .
W1 O2 W3 95.9(4) . .
Sb1 O2 W2 128.1(5) . .
W1 O2 W2 95.0(4) . .
W3 O2 W2 91.9(4) . .
W1 O3 Fe1 168.9(7) . .
W1 O4 Fe2 165.2(7) . 2_666
O5' O5 W3 63(4) . .
O5' O5 W1 93(4) . .
W3 O5 W1 119.9(6) . .
O5 O5' W3 91(4) . .
O5 O5' W1 66(4) . .
W3 O5' W1 120(3) . .
O6' O6 W2 73(4) . .
O6' O6 W1 72(4) . .
W2 O6 W1 119.4(7) . .
O6 O6' W2 83(5) . .
O6 O6' W1 87(4) . .
W2 O6' W1 128(3) . .
W2 O8 W7 146.6(7) . .
W6 O9 W2 144.0(6) . .
O10' O10 W3 84(4) . .
O10' O10 W2 83(4) . .
W3 O10 W2 119.4(6) . .
O10 O10' W3 71(3) . .
O10 O10' W2 72(4) . .
W3 O10' W2 111(2) . .
W5 O12 W3 145.8(7) . .
W3 O13 W4 146.5(6) . .
Sb1 O14 W5 137.9(5) . .
Sb1 O14 W9 113.3(4) . .
W5 O14 W9 95.3(4) . .
Sb1 O14 W4 114.7(5) . .
W5 O14 W4 92.8(4) . .
W9 O14 W4 93.0(4) . .
W9 O16 W4 119.5(6) . .
W4 O17 Fe1 142.3(6) . 2_666
W5 O18 W4 117.9(6) . .
W5 O19 Sm1 150.0(7) . .
W5 O20 W9 120.1(6) . .
W5 O21 W6 155.1(7) . .
Sb1 O23 W8 113.6(5) . .
Sb1 O23 W7 114.8(6) . .
W8 O23 W7 94.2(4) . .
Sb1 O23 W6 137.9(5) . .
W8 O23 W6 94.8(4) . .
W7 O23 W6 92.0(4) . .
W6 O24 W8 118.8(6) . .
W6 O25 W7 118.0(6) . .
W7 O27 W8 117.7(5) . .
W7 O28 Fe1 144.9(7) . .
W8 O30 W9 146.9(7) . .
W8 O31 Fe2 134.2(7) . .
W9 O33 Fe2 138.0(6) . .
O7W Sm1 O8W 62.1(9) . .
O7W Sm1 O11W 138.2(10) . .
O8W Sm1 O11W 77.7(9) . .
O7W Sm1 O12W 142.5(9) . .
O8W Sm1 O12W 135.2(7) . .
O11W Sm1 O12W 75.4(9) . .
O7W Sm1 O9W 68.5(9) . .
O8W Sm1 O9W 98.4(8) . .
O11W Sm1 O9W 132.6(9) . .
O12W Sm1 O9W 75.4(8) . .
O7W Sm1 O5W 58.5(9) . .
O8W Sm1 O5W 82.1(8) . .
O11W Sm1 O5W 107.1(9) . .
O12W Sm1 O5W 140.2(8) . .
O9W Sm1 O5W 119.3(8) . .
O7W Sm1 O6W 83.9(8) . .
O8W Sm1 O6W 145.2(7) . .
O11W Sm1 O6W 132.7(8) . .
O12W Sm1 O6W 76.7(7) . .
O9W Sm1 O6W 73.7(7) . .
O5W Sm1 O6W 73.4(8) . .
O7W Sm1 O19 126.6(8) . .
O8W Sm1 O19 125.2(6) . .
O11W Sm1 O19 67.8(7) . .
O12W Sm1 O19 75.1(6) . .
O9W Sm1 O19 136.3(6) . .
O5W Sm1 O19 69.9(7) . .
O6W Sm1 O19 68.6(5) . .
O7W Sm1 O10W 100.2(11) . .
O8W Sm1 O10W 60.8(9) . .
O11W Sm1 O10W 67.0(10) . .
O12W Sm1 O10W 75.8(9) . .
O9W Sm1 O10W 70.1(10) . .
O5W Sm1 O10W 142.9(9) . .
O6W Sm1 O10W 138.8(9) . .
O19 Sm1 O10W 130.7(8) . .
O33 Fe2 O4 97.1(5) . 2_666
O33 Fe2 O31 87.7(5) . .
O4 Fe2 O31 96.5(5) 2_666 .
O33 Fe2 O34 90.7(5) . .
O4 Fe2 O34 169.6(5) 2_666 .
O31 Fe2 O34 90.6(5) . .
O33 Fe2 O3W 92.0(6) . .
O4 Fe2 O3W 86.9(5) 2_666 .
O31 Fe2 O3W 176.6(5) . .
O34 Fe2 O3W 86.0(5) . .
O33 Fe2 O4W 174.3(5) . .
O4 Fe2 O4W 87.9(5) 2_666 .
O31 Fe2 O4W 89.0(6) . .
O34 Fe2 O4W 84.6(5) . .
O3W Fe2 O4W 91.0(7) . .
C1 O34 Fe2 141(2) . .
C1 O35 H35A 109.5 . .
C3 O36 H36A 109.5 . .
C2 N1 H1A 120.0 . .
C2 N1 H1B 120.0 . .
H1A N1 H1B 120.0 . .
O34 C1 O35 132(4) . .
O34 C1 C2 121(3) . .
O35 C1 C2 106(3) . .
C3 C2 N1 127(4) . .
C3 C2 C1 110(3) . .
N1 C2 C1 101(3) . .
C3 C2 H2A 105.7 . .
N1 C2 H2A 105.7 . .
C1 C2 H2A 105.7 . .
C2 C3 O36 104(3) . .
C2 C3 C4 105(3) . .
O36 C3 C4 100(3) . .
C2 C3 H3A 115.2 . .
O36 C3 H3A 115.2 . .
C4 C3 H3A 115.2 . .
C3 C4 H4A 109.5 . .
C3 C4 H4D 109.5 . .
H4A C4 H4D 109.5 . .
C3 C4 H4B 109.5 . .
H4A C4 H4B 109.5 . .
H4D C4 H4B 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sb1 O14 1.994(11) .
Sb1 O23 1.997(11) .
Sb1 O2 2.012(10) .
W1 O4 1.772(13) .
W1 O3 1.784(12) .
W1 O1 1.808(12) .
W1 O6' 1.94(5) .
W1 O5 2.024(13) .
W1 O6 2.038(13) .
W1 O5' 2.22(6) .
W1 O2 2.234(11) .
W2 O7 1.724(12) .
W2 O6' 1.80(5) .
W2 O6 1.865(14) .
W2 O8 1.870(11) .
W2 O9 1.957(11) .
W2 O10 1.960(13) .
W2 O10' 2.05(5) .
W2 O2 2.339(11) .
W3 O5' 1.67(5) .
W3 O11 1.721(12) .
W3 O5 1.882(14) .
W3 O13 1.913(12) .
W3 O10 1.916(13) .
W3 O12 1.959(12) .
W3 O10' 2.02(5) .
W3 O2 2.319(11) .
W4 O15 1.722(12) .
W4 O17 1.828(12) .
W4 O18 1.928(11) .
W4 O16 1.931(12) .
W4 O13 1.949(12) .
W4 O14 2.296(10) .
W5 O19 1.736(13) .
W5 O12 1.889(12) .
W5 O21 1.892(11) .
W5 O20 1.913(12) .
W5 O18 1.925(11) .
W5 O14 2.261(10) .
W6 O22 1.715(11) .
W6 O25 1.899(13) .
W6 O9 1.904(11) .
W6 O21 1.912(11) .
W6 O24 1.920(11) .
W6 O23 2.323(11) .
W7 O26 1.692(12) .
W7 O28 1.821(11) .
W7 O27 1.909(11) .
W7 O25 1.974(12) .
W7 O8 1.981(11) .
W7 O23 2.291(12) .
W8 O29 1.746(11) .
W8 O31 1.814(11) .
W8 O30 1.889(13) .
W8 O27 1.974(12) .
W8 O24 1.987(11) .
W8 O23 2.244(12) .
W9 O32 1.737(12) .
W9 O33 1.843(12) .
W9 O16 1.924(11) .
W9 O20 1.972(12) .
W9 O30 1.972(12) .
W9 O14 2.294(10) .
Fe1 O28 1.923(11) .
Fe1 O17 1.937(12) 2_666
Fe1 O3 1.953(12) .
Fe1 O1 1.956(12) 2_666
Fe1 O2W 2.087(12) .
Fe1 O1W 2.087(12) .
O5W Sm1 2.47(2) .
O6W Sm1 2.474(16) .
O7W Sm1 2.42(3) .
O8W Sm1 2.42(2) .
O9W Sm1 2.459(19) .
O10W Sm1 2.51(3) .
O11W Sm1 2.44(2) .
O12W Sm1 2.452(18) .
O23W O22W 1.49(7) 2_666
O22W O23W 1.49(7) 2_666
O1 Fe1 1.956(12) 2_666
O4 Fe2 1.983(13) 2_666
O5 O5' 0.83(6) .
O6 O6' 0.74(5) .
O10 O10' 0.86(5) .
O17 Fe1 1.937(12) 2_666
O19 Sm1 2.486(14) .
O31 Fe2 1.986(13) .
O33 Fe2 1.919(12) .
Fe2 O4 1.983(13) 2_666
Fe2 O34 2.048(13) .
Fe2 O3W 2.063(12) .
Fe2 O4W 2.078(14) .
O34 C1 1.03(4) .
O35 C1 1.30(4) .
O35 H35A 0.8200 .
O36 C3 1.51(4) .
O36 H36A 0.8200 .
N1 C2 1.472(10) .
N1 H1A 0.8600 .
N1 H1B 0.8600 .
C1 C2 1.64(5) .
C2 C3 1.44(4) .
C2 H2A 0.9800 .
C3 C4 1.70(6) .
C3 H3A 0.9800 .
C4 H4A 0.9600 .
C4 H4D 0.9600 .
C4 H4B 0.9600 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O35 H35A O4W 0.82 2.37 3.04(3) 139.6 .
O35 H35A O25W 0.82 2.40 3.08(3) 140.8 2_656
O36 H36A O24W 0.82 1.73 2.50(4) 156.1 2_666
O36 H36A O12W 0.82 2.30 2.78(3) 117.7 2_655
N1 H1A O22W 0.86 2.27 3.12(8) 170.9 2_655
N1 H1B O30 0.86 2.32 3.07(4) 145.7 .
N1 H1B O29 0.86 2.38 3.06(4) 136.6 .
